# Raw materials and their characterization

```2. Shaping
2.0 Introduction
In classical ceramic technology forming or shaping is the process step to transform a ceramic
powder (raw materials mixture) into a weakly bound powder compact (green body). Prior to
shaping: comminution (e.g. milling), mixing (e.g. with water or another temporary vehicle
phase, which is later eliminated) and / or granulation (e.g. by spray drying). After shaping:
drying and / or debinding and firing. Note that the final microstructure of the sintered ceramic
body is determined by the green microstructure adopted during shaping and that defects
introduced during shaping usually cannot be eliminated in subsequent processing steps. For
shaping techniques using liquid vehicles (aqueous or organic) the volume fraction of powder
geometrical tolerances and minimize shrinkage and deformation  optimal deagglomeration
and deflocculation necessary in the suspension (slurry, slip or paste). For dry pressing
methods granulated powders are preferred because of easier mold filling with free-flowing
powders. For a monosized spherical particle the maximum packing fraction is approx. 64 %
(random close packing). Mathematical modeling of the body-formation kinetics of traditional
slip-casting exploits Fick’s law (and or Darcy’s law), while the velocity profiles in extrusion
can be modeled using the momentum balance in combination with an appropriate constitutive
equation (e.g. the Herschel-Bulkley relation for generalized viscoplastic pastes).
2.1 Dry pressing


Die pressing: usually for small and simple shapes made from granulated powders;
the mold wall due to frictional resistance, especially for unidirectional die pressing,
i.e. piston movement only from one side)  non-uniformities (lamination) in the
microstructure; to minimize this problem: bidirectional die pressing (piston
countermovement from two sides).
Cold isostatic pressing (CIP): for larger and more complex shapes (but not too large
and not too complicated); hydrostatic pressure exerted by a liquid medium in all
directions (wet bag CIP using a rubber mold) or at least radially (dry bag CIP)  less
density gradients; pressures commonly up to 200 MPa (in wet bag presses for large
bodies up to 500 MPa).
2.2 Plastic forming


Jiggering, roller-tool forming of plastic or semi-dry masses (for thin-wall shapes with
rotational symmetry) typical for tableware; roll compaction (for 2D ceramic sheets).
Extrusion (for translationally symmetric shapes, large or small): viscoplastic pastes
(with a yield stress and apparent viscosity of several Pas to several kPas) are shaped
by pressure-driven flow through an orifice  radial density gradients and / orientation
textures; pressure exerted by auger or piston; wide product range from traditional
coarse ceramics (profiled clay-based bricks, using water) to advanced fine ceramics
(alumina or cordierite honeycomb catalyst supports, using organic vehicles; when
organics are used  defect-free burnout before firing is a critical step); co-extrusion
can be used to produce laminates or unidirectional composites.

Injection molding (for small parts with complex geometries): ceramic powder
feedstock with binder (usually polymer- or wax-based); upon heating the binder
liquefies; after mold filling (injection) the binder solidifies  green part can be
ejected (but requires sufficiently slow binder burnout before sintering, usually in the
temperature range 300–700 °C; this processing step is size-limiting); capital-expensive
technique (economically useful only for mass production); hot molding (low-pressure
variant of injection molding for feedstocks with lower apparent viscosity).
2.3 Casting techniques



Slip casting and pressure slip-casting (preferentially for thin-walled bodies, large or
small): body formation by dewatering (drainage) of highly fluid slips (apparent
viscosity < 500 mPas) across a semipermeable mold wall (plaster or porous polymer);
body formation kinetics obey a square-root-of-time law  microstructural gradients
are possible from the body interior to the wall. The related techniques centrifugal
casting and electrophoretic deposition usually exhibit enhanced density gradients and
can be applied to produce functionally graded materials using a slip-casting approach.
Gel casting and related techniques, e.g. direct coagulation casting (DCC) use a
(thermally or chemically induced) in-situ phase transition (e.g. a gelling transition) of
an organic or water-based vehicle and enables casting of suspensions into non-porous
molds (e.g. metal molds)  uniform (i.e. gradient-free) microstructure; a similar
process is starch consolidation casting (SCC), based on the ability of starch to swell in
water at elevated temperature (starch used as a pore-forming and body-forming agent).
Tape casting (typical thickness several hundred µm): ceramic suspension (containing
binder, plasticizer, solvents and functional additives) deposited on a flat carrier
substrate, results in 2D ceramic sheets after firing (e.g. for multilayer capacitors).
2.4 Other techniques


Hot pressing: compaction and sintering of green bodies at the same time; mechanical
pressure > 20 MPa increases the driving force for densification (by acting against the
internal pore pressure) without increasing the driving force for grain growth 
reduced sintering temperature to achieve high density and fine grain size; commonly
used to sinter high-purity products normally requiring high sintering temperatures and
/ or sintering additives (which would deteriorate properties).
Hot isostatic pressing (HIP): pressure 10–200 MPa exerted by hot pressurized gas;
product size should not be too large, product shape should not be too complicated; can
also be used as a post-sintering technique to reduce the size of closed pores; expensive
technique (useful only for high-value products designed for demanding applications).
Complex exercise problem: Discuss the results of mathematical modeling of extrusion
processes for composite ceramics (particulate-, platelet- and fiber/whisker-reinforced) in
relation to the evolving microstructure, with special regard to particle shape. Further, discuss
the question of microstructural uniformity in other shaping processes, especially in the new
shaping methods gel casting and starch consolidation casting. Additional explicit questions:
a.) What is the underlying reason for microstructural non-uniformity in extrusion
processes ? Make a clear distinction between material and process parameters.
b.) How can texture effects generally be avoided ? By what methods can anisotropic or
non-uniform (functionally graded) ceramics be produced ?
```
##### Related flashcards
Materials science

63 Cards

Acoustics

44 Cards